Effect of nanoparticles on heat capacity of nanofluids based on molten salts as PCM for thermal energy storage
© Chieruzzi et al.; licensee Springer. 2013
Received: 5 August 2013
Accepted: 13 October 2013
Published: 29 October 2013
In this study, different nanofluids with phase change behavior were developed by mixing a molten salt base fluid (selected as phase change material) with nanoparticles using the direct-synthesis method. The thermal properties of the nanofluids obtained were investigated. These nanofluids can be used in concentrating solar plants with a reduction of storage material if an improvement in the specific heat is achieved. The base salt mixture was a NaNO3-KNO3 (60:40 ratio) binary salt. The nanoparticles used were silica (SiO2), alumina (Al2O3), titania (TiO2), and a mix of silica-alumina (SiO2-Al2O3). Three weight fractions were evaluated: 0.5, 1.0, and 1.5 wt.%. Each nanofluid was prepared in water solution, sonicated, and evaporated. Measurements on thermophysical properties were performed by differential scanning calorimetry analysis and the dispersion of the nanoparticles was analyzed by scanning electron microscopy (SEM). The results obtained show that the addition of 1.0 wt.% of nanoparticles to the base salt increases the specific heat of 15% to 57% in the solid phase and of 1% to 22% in the liquid phase. In particular, this research shows that the addition of silica-alumina nanoparticles has a significant potential for enhancing the thermal storage characteristics of the NaNO3-KNO3 binary salt. These results deviated from the predictions of the theoretical model used. SEM suggests a greater interaction between these nanoparticles and the salt.
KeywordsPhase change materials Nanofluid Thermal energy storage Nanoparticles Heat capacity Molten salt Nanocomposite
The growing world energy demand  is increasing the burning of fossil fuels and, consequently, the carbon dioxide emissions. In order to limit these emissions, it is necessary to make better use of the produced thermal energy by increasing the energy efficiency of industrial processes (heat recovery) and buildings and the use of renewable sources such as solar energy .
Economic storage of thermal energy (thermal energy storage - TES) is a key technological issue for solar thermal power plants and industrial waste heat recovery [3–5]. The overall objectives of heat storage integration are to increase the solar contribution, to improve efficiency, and to reduce the levelized energy cost (LEC). TES systems can be used at high temperature (T > 400°C) or at lower temperature (ranging from 100°C to about 300°C) for heat and solar cooling. Low-temperature storage systems are based almost entirely on sensible heat storage using liquid water , but for temperatures exceeding 100°C (concentrated solar power plants), non-pressurized liquid water and the use of pressure vessels make this technology unattractive.
Among the various methods of energy storage, latent heat thermal energy storage (LHTES) systems using phase change materials (PCMs) have been gaining importance in such fields as solar energy systems, district heating and cooling systems, energy efficiency buildings [6–9], cool storage systems for central air-conditioning systems, and waste heat recovery systems . This is mainly due to their high energy storage density and their ability to provide heat at a constant temperature. Since the latent heat of fusion between the liquid and solid phases of PCMs is high compared to sensible heat, storage systems utilizing PCMs can be reduced in size with respect to systems based on sensible heat. Therefore, several studies on PCM used as thermal energy storage material have been published [10–16].
The materials needed for phase-change thermal energy storage must have a large latent heat and high thermal conductivity. They should have a melting temperature lying in the practical range of operation, offer chemical stability and they should be low cost, nontoxic, and non-corrosive. PCMs studied during the last 40 years are mainly paraffin waxes, fatty acids, metal alloys, salts (fluorides and chlorides, hydroxides, nitrates, carbonates) [17–20]. There are many LHTES systems used in practical applications. They can be composed of PCM elements with similar shapes such as PCM spheres, PCM cylinders, PCM flat plates or even PCM capsules with irregular shapes .
Some researchers have shown that the addition of nanoparticles may allow an increase in both the thermal capacity and the thermal conductivity of the storage media [21–23]. The concept of nanofluid as a fluid with nanoparticles suspended by Brownian motion was introduced in 1995 by Choi who showed an increase in thermal properties of some fluids after the addition of copper or aluminum nanoparticles . The increase of these properties can be considerably enhanced by a small amount of nanoparticles added to the storage media with obvious advantages for the thermal energy storage systems. In fact, a high thermal capacity allows storing a high quantity of heat in a small volume of material. This allows the realization of compact thermal storage systems with the advantage to limit energy losses (reducing the outer exchanging surfaces) and, above all, to reduce costs.
However, research work on the specific heat of nanofluids has been limited compared to that on thermal conductivity especially those prepared by adding nanoparticles [21, 25–29]. Nevertheless, it is essential to evaluate the heat capacity of these nanofluids since an improvement in the specific heat can reduce the amount of storage material.
The aim of this work is the development of a new phase change material using different kinds of nanoparticles embedded in a molten salt base material and the thermal characterization of the nanofluid obtained.
A binary nitrate salt, widely used in liquid phase as sensible heat storage media in high temperature solar plants (solar salt), has been selected as PCM. This salt is a mixture of 60% NaNO3 and 40% KNO3 which has a melting point of about 220°C. This melting temperature is useful for many medium-low power applications . The salts were purchased from Sigma-Aldrich (St. Louis, MO, USA). The selected nanoparticles were silica (Aerosil300, average diameter 7 nm, Evonik Industries, Hanau-Wolfgang Germany), alumina (Aeroxide AluC, average diameter 13 nm), a hydrophilic fumed mixed oxide of silica (82% to 86%) and alumina (14% to 18%) (Aerosil Cok84, average diameter 2 to 200 nm) supplied by Evonik and titania (titanium dioxide, 99.97% average diameter 20 nm) supplied by Sigma-Aldrich.
The binary salt was prepared by mixing 60 parts of NaNO3 with 40 parts of KNO3 in solid state, then heating them at 300°C to achieve a complete melting and mixing of the two salts. The system was then cooled at room temperature and a white solid mixture was obtained. The solid binary salt was then milled to powder and immediately used. The nanoparticles were dispersed into three concentrations: 0.5, 1.0, and 1.5 wt.%. The procedure followed to prepare the nanofluids consists of four steps: 198 mg of NaNO3-KNO3 and 2 mg of nanoparticles (related in this case to 1.0 wt.% of nanoparticles) were measured on an analytical balance with ±0.1-mg precision (Mettler Toledo, type AB104-S, Greifensee, Switzerland); the binary salt and the nanoparticles were dispersed in 20 ml of distilled water by ultrasonic mixing for 100 min (Ultrasonic bath, EMMEGI mod.AC-5, Milan, Italy); afterwards, the water solution was heated at 200°C on a hot plate to fully remove the water (for at least 2 h) . The same procedure was followed to prepare the nanofluids with 0.5 and 1.5 wt.% of nanoparticles and to prepare the neat molten salt for comparison with the nanofluids obtained. The nanofluids were formulated without the use of any dispersant/surfactant. All the materials used in this work were subjected to dehydration in order to remove all the water entrapped. After this operation, they were immediately used for DSC analysis. In this way, we avoided any possible negative effect of the water.
Differential scanning calorimetry
Differential scanning calorimetry (DSC) tests were performed on a Mettler-Toledo DSC 822E/400. The dry samples obtained after water evaporation were introduced in standard aluminum pans with lid and subjected to the following thermal cycle in nitrogen atmosphere: held at 150°C for 5 min (to remove any absorbed water in the sample), heating from 150°C to 300°C at 20°C/min, held at 300°C for 5 min, cooling from 300°C to 150°C at 20°C/min. Six consecutive cycles were run on each sample without opening the DSC furnace to ensure good mixing of the sample and reproducibility of the results. In this way, the effect of the initial granulometry was also lost after the first cycles. The DSC thermograms were analyzed and the phase-change heat and melting temperatures were obtained using the software STARe. Moreover, the calorimetric data were used to calculate the specific heat (Cp) of the samples.
Same scanning tests were performed on the base salt and the melting properties compared with those obtained with the nanofluids. In this way, the effect of the different nanoparticles could be evaluated.
In particular, the DSC procedure followed to estimate specific heat values was the three-step procedure . First of all, a thermal cycle was fixed. In the first step, a measurement was taken with two empty sample pans. During this measurement, the baseline heat flux (Q0) was obtained. The results of this measurement indicate the bias in the DSC. In the second step, a pan containing the reference sample with a known specific heat and an empty pan were loaded into the calorimeter. The heat flux recorded was Qref. In the third step, a pan containing the sample and an empty pan were loaded into the calorimeter. The heat flux into the sample (Qsample) was recorded. The specific heat of the sample was obtained as follows: Cp,sample = [(Qsample−Q0)/(Qref−Q0)] × (mref−msample) × Cp,ref, where mref and msample indicate the masses of the reference and sample, respectively.
This procedure was validated with our base fluid whose specific heat is well known.
where Cp is specific heat, ∅ is the volume fraction, ρ is the density, and the subscripts np, nf, and f refer to nanoparticle, nanofluid, and base fluid, respectively.
Scanning electron microscopy
The morphological analysis of the samples was performed with a field emission scanning electron microscope (FESEM model SUPRA25, ZEISS, Oberkochen, Germany). One specimen for each system after DSC measurement was analyzed in order to evaluate the dispersion of the nanoparticles. Each sample was metallized with a thin layer of gold (15 nm, 99.99% of gold, 2 × 10−6 Torr) in a thermal evaporator (Sistec thin film equipment model GP 20 by Kenosistec Angelantoni Group, Massa Martana (PG), Italy). For the surface analysis, secondary electrons were used. SEM analysis has been used in other works focused in the preparation and characterization of nanofluids to evaluate the dispersion/aggregation of nanoparticles [21, 22, 32].
Moreover, a recent study analyzed the aggregation of nanoparticles in the same base fluid studied in our work using the SEM technique .
Results and discussion
Heat of fusion, melting temperature, and onset temperature of NaNO 3 -KNO 3 (60:40) mixture and nanofluids obtained with different nanoparticles
Nanoparticle concentration (wt.%)
Heat of fusion (kJ/kg)
Onset temperature (°C)
Melting temperature (°C)
Base salt mixture
Base salt + SiO2
Base salt + Al2O3
Base salt + TiO2
Base salt + SiO2-Al2O3
In particular, the analyzed binary salt and the nanofluids obtained by adding nanoparticles in the binary salt, are not pure materials; therefore, instead of a melting temperature, they show a range of melting temperatures. The onset and the melting temperatures were both taken because the complete phase transformation is not reached at the onset temperature but only above the melting temperature. In fact, above this temperature, the salt mixture and the nanofluids are completely liquid and can be used as fluids for solar energy storage. For this reason, the melting temperature was taken as the real melting point of the salt mixture and the nanofluids and the two characteristic temperatures were both useful to describe the melting behavior of PCMs.
The onset temperature of the endothermic peak for the binary salt was 219.8°C while the melting temperature was 232.01°C. The addition of the four types of nanoparticles lead to a reduction of onset temperatures and melting points. This effect was found for all the three concentrations investigated but it was more evident for 1.0 wt.% of nanoparticles added. In particular, the addition of 1.0 wt.% of SiO2-Al2O3 lead to a maximum Tonset decrease of 5% with respect to the base salt mixture (i.e., about 10°C).
In particular, the onset temperature decreased by adding SiO2, Al2O3, TiO2, and SiO2-Al2O3. This means that the phase change occurs at a lower temperature with respect to the base salt with a clear advantage when used in solar plants.
Moreover, also the phase-change temperature was lowered by adding the selected nanoparticles to the NaNO3-KNO3 salt mixture, especially with 1.0 wt.% of SiO2-Al2O3. In this case, the melting point decreased by more than 8°C. For the other nanofluids, the decrease in melting temperature was slightly modified (<1%).
A higher effect of the addition of nanoparticles was obtained on the latent heat. In particular, adding 1.0 wt.% of the nanoparticles produced an enhancement of the heat of fusion by more than 15% for almost all the nanofluids obtained. Only the nanofluid based on TiO2 produced an increment of 5%. Even in this case, 1.0 wt.% of SiO2-Al2O3 produced the higher enhancement. This means that the nanoparticles added to the base salt mixture allow the heat storage to be more effective per unit volume.
The addition of nanoparticles influenced also the heat capacity in solid and liquid phases. The specific heats were calculated as average of single values recorded in the temperature range 155°C to 220°C (where 220°C is about the onset temperature) in solid phase and in the range 250°C to 300°C (where 250°C is about the endset temperature) in liquid phase (the endset temperature is the intersection point of the baseline after transition and the inflectional tangent).
Specific heat of NaNO 3 -KNO 3 (60:40) mixture and nanofluids obtained with different nanoparticles
Nanoparticle concentration wt.%
Specific heat (solid phase; kJ/kg·K)
Enhancement (solid phase; %)
Specific heat (liquid phase; kJ/kg·K)
Enhancement (liquid phase; %)
Base salt mixture
Base salt + SiO2
Base salt + Al2O3
Base salt + TiO2
Base salt + SiO2-Al2O3
Furthermore, the Cp increase obtained with the addition of 1.0 wt.% of SiO2-Al2O3 nanoparticles was undoubtedly the most important among all the characterized mixtures (57% in solid phase and 22% in liquid phase).
The reduction in the specific heat capacity of the nanofluids obtained from the model is clearly explained since oxide nanoparticles show lower specific heats with respect to the base phase change material. This behavior was also reported in previous studies [21, 26, 35, 36].
Moreover, the values of Cp experimentally evaluated for 1.0 wt.% of nanoparticles resulted much higher than the theoretical values. This different behavior was explained by admitting the existence of other mechanisms for nanofluids . Different mechanisms were proposed to explain the enhancement of thermal conductivity; it is possible to suppose that the same mechanisms could be used to explain the enhancement of specific heat. They are based on Brownian motion of nanoparticles [37–39], aggregation of nanoparticles [40–42] and formation of a nanolayer [21, 43–45].
In our work, the observed enhancement of heat capacity was not related to the presence of a substructure. In any case, since it was shown that the specific heat is a structure-insensitive property , the formation of networks in the structure of nanofluids should not affect the specific heat.
In addition, the Brownian motion of nanoparticles should not be responsible for the enhancement since heat capacity is not a transport property. On the other hand, the agglomeration of nanoparticles and the formation of clusters can increase the thermal conductivity but, in our work, does not seem to have the same effect on the specific heat.
The most significative mechanism that led to an increment of Cp could be considered the formation of a solid-like nanolayer on the surface of the nanoparticle. This layer has higher thermal properties than the bulk liquid contributing in this way to the increase of specific heat of nanofluids [21, 33].
The kinetic effect was taken into account in calorimetric analysis. The scanning rate adopted was 20°C/min because it was the heating rate commonly used for specific heat evaluation. Moreover, faster program rates seem to improve also the accuracy of specific heat evaluation . DSC tests at 10°C/min were also performed and a difference of about 6% in Cp was found.
The area enclosed by a curve of the nanofluid and the curve of the base salt provided an indication of how much the thermal capacity of the new storage medium was increased. The curves related to the nanofluids with 0.5 wt.% and 1.5 wt.% of nanoparticles were lower than the base salt curve. On the contrary, the curves of stored heat versus temperature for the nanofluids with 1.0 wt.% of nanoparticles were above the base salt curve. Even in this case, it was evident the higher increase of the thermal capacity obtained with the addition of 1.0 wt.% SiO2-Al2O3 nanoparticles. The total gain due to the introduction of the nanoparticles was given by the ratio between the total stored heat of the nanofluids and the total stored heat of the base salt mixture. The stored heat as function of temperature avoids the definition of a single melting temperature, a constant heat capacity that might not exist, as well as the separation between sensible heat and latent heat .
The morphological characterization was carried on in order to evaluate the degree of dispersion of the nanoparticles in the nanofluid after the calorimeter cycle test was performed. SEM analysis was useful to understand the factors that are responsible of the improvement of the Cp. In fact, it is assumed that a uniform distribution and a homogeneous dispersion of the filler contribute to higher Cp values and lower melting points of the nanofluid.
The agglomeration observed in the nanofluids could be caused by variations in pH during the synthesis of nanofluids, variations in concentration or temperature cycling . Moreover, the distribution of nanoparticles in the base fluid could be improved using surfactants to break down the particle conglomeration in suspension . This is the subject of future work by our research group.
The SEM characterization of the nanofluids developed in our study did not show the presence of a substructure at nanoparticle locations as reported in other researches [21, 32] that was considered as probably responsible for heat capacity enhancement. Nevertheless, the higher specific heat recorded in our research could be associated to the high specific surface energies associated with the high surface area of the nanoparticles per unit volume [51, 52]. Moreover, the higher enhancement obtained with SiO2-Al2O3 nanoparticles could be potentially due to the large distribution of nanoparticle size from 2 to 200 nm. This also implies the presence of smaller nanoparticles with respect to the other additives. Nanoparticles with a smaller diameter could be more effectively dispersed into the salt and give better thermal characteristics [53, 54]. The size of nanoparticles, in fact, defines the surface-to-volume ratio and the suspension of smaller particles has a greater area of the solid/liquid interface (for the same volume concentrations). Hence, the contribution of interfacial effects will be stronger in this kind of suspensions [55, 56].
High-temperature nanofluids with the addition of different kinds of nanoparticles to a binary salt (NaNO3-KNO3 with a 60:40 ratio) with PCM behavior were studied. The nanoparticles added were silica, alumina, titania, and a mixture of silica-alumina. Three weight fractions were studied (0.5, 1.0, and 1.5 wt.%). The nanofluids obtained were subjected to calorimetry and the dispersion of the nanoparticles was analyzed by SEM. The effect on nanoparticle concentration was also investigated.
DSC showed that the addition of nanoparticles to base salt increased the heat of fusion of the nanofluid compared to the observed heat of fusion of the unmodified base salt (with the higher increase obtained with 1.0 wt.%). The onset temperature and the melting temperature were lowered by the addition of all nanoparticles. Moreover, there was an increase of Cp with the addition of 1.0 wt.% of nanoparticles. In particular, the best results were obtained with the addition of 1.0 wt.% of SiO2-Al2O3 that showed a decrease of more than 8°C for the melting point and 10°C for the onset temperature and higher enhancement of the specific heat capacity of the salt mixture (57% in solid phase and 22% in liquid phase).
SEM images suggest a higher interaction between the SiO2-Al2O3 nanoparticles and the salt especially with 1.0 wt.% of nanoparticles. This work demonstrates that an increase in specific heat is achievable with the use of nanoparticles with relevant advantages for thermal storage. In general, concentrations lower and higher than 1.0 wt.% did not show the same enhancement of thermal properties. Moreover, the observed enhancements are suggested to be due to the high specific surface energies associated with the high surface area of the nanoparticles per unit volume.
The enhanced specific heat capacity of the nanofluids can significantly reduce the required amount of thermal energy storage media in concentrated solar power plants with a consequent reduction in the cost of electricity.
Thermal energy storage
Latent heat thermal energy storage
Phase change material
Differential scanning calorimetry
Scanning electron microscopy.
The authors would like to thank the Italian National Agency for New Technologies, Energy and Sustainable Economic Development for the financial support of this research.
- International Energy Agency IEA: World Energy Outlook 2011. Paris; 2011.Google Scholar
- International Energy Agency IEA: Technology Roadmap: Solar Heating and Cooling. Paris; 2012.Google Scholar
- Hasnain SM: Review on sustainable thermal energy storage technologies, Part I: Heat Storage Materials and techniques. Energ Convers Manage 1998, 39(11):1127–1138. 10.1016/S0196-8904(98)00025-9View ArticleGoogle Scholar
- Herrmann U, Kearney DW: Survey of thermal energy storage for parabolic trough power plants. J Sol Energy Eng 2002, 124(2):145–152. 10.1115/1.1467601View ArticleGoogle Scholar
- Laing D: Solar thermal energy storage technologies. In Energy Forum 10000 Solar Gigawatts, 23 April 2008. Hannover: Hannover Messe; 2008. http://www.dlr.de/Portaldata/41/Resources/dokumente/institut/thermischept/Solar_Thermal_Energy_Storage_Technologies_Hannover2008.pdfGoogle Scholar
- Gil A, Medrano M, Martorell I, Lazaro A, Dolado P, Zalba B, Cabeza LF: State of the art on high temperature thermal energy storage for power generation. Part 1-Concepts, materials and modellization. Renew Sust Energ Rev 2010, 14: 31–55. 10.1016/j.rser.2009.07.035View ArticleGoogle Scholar
- Cabeza LF, Castell A, Barreneche C, de Gracia A, Fernández AI: Materials used as PCM in thermal energy storage in buildings: a review. Renew Sust Energ Rev 2011, 15: 1675–1695. 10.1016/j.rser.2010.11.018View ArticleGoogle Scholar
- Baetens R, Jelle BP, Gustavsen A: Phase change materials for building applications: a state-of-the-art review. Energ Buildings 2010, 42: 1361–1368. 10.1016/j.enbuild.2010.03.026View ArticleGoogle Scholar
- Kuznik F, David D, Johannes K, Roux J: A review on phase change materials integrated in building walls. Renew Sust Energ Rev 2011, 15: 379–391. 10.1016/j.rser.2010.08.019View ArticleGoogle Scholar
- Sharma A, Tyagi VV, Chen CR, Buddhi D: Review on thermal energy storage with phase change materials and applications. Renew Sust Energ Rev 2009, 13: 318–345. 10.1016/j.rser.2007.10.005View ArticleGoogle Scholar
- Sharma SD, Sagara K: Latent heat storage materials and systems: a review. Int J Green Energy 2005, 2: 1–56. 10.1081/GE-200051299View ArticleGoogle Scholar
- Tamme R, Bauer T, Buschle J, Laing D, Muller-Steinhagen H, Steinmann WD: Latent heat storage above 120°C for applications in the industrial process heat sector and solar power generation. Int J Energ Res 2008, 32: 264–271. 10.1002/er.1346View ArticleGoogle Scholar
- Sarı A, Karaipekli A: Preparation, thermal properties and thermal reliability of palmitic acid/expanded graphite composite as form-stable PCM for thermal energy storage. Sol Energ Mat Sol C 2009, 93: 571–576. 10.1016/j.solmat.2008.11.057View ArticleGoogle Scholar
- Farid MM, Khudhair AM, Razack SAK, Al-Hallaj S: A review on phase change energy storage: materials and applications. Energ Convers Manage 2004, 45: 1597–1615. 10.1016/j.enconman.2003.09.015View ArticleGoogle Scholar
- Zalba B, Marın JM, Cabeza LF, Mehling H: Review on thermal energy storage with phase change: materials, heat transfer analysis and applications. Appl Therm Eng 2003, 23: 251–283. 10.1016/S1359-4311(02)00192-8View ArticleGoogle Scholar
- Kenisarin MK: High-temperature phase change materials for thermal energy storage. Renew Sust Energ Rev 2010, 14: 955–970. 10.1016/j.rser.2009.11.011View ArticleGoogle Scholar
- Araki N, Matsuura M, Makino A, Hirata T, Kato Y: Measurement of thermophysical properties of molten salts: mixtures of alkaline carbonate salts. Int J Thermophys 1988, 9: 1071–1080. 10.1007/BF01133274View ArticleGoogle Scholar
- Rozanna D, Chuah TG, Salmiah A, Choong TSY, Sa’ari M: Fatty acids as phase change materials (PCMs) for thermal energy storage: a review. Int J Green Energy 2004, 1(4):495–513.View ArticleGoogle Scholar
- Akgün M, Aydın O, Kaygusuz K: Experimental study on melting/solidification characteristics of a paraffin as PCM. -. Energ Convers Manage 2007, 48: 669–678. 10.1016/j.enconman.2006.05.014View ArticleGoogle Scholar
- Farkas D, Birchenall CE: New eutectic alloys and their heats of transformation. Metall Trans A 1985, 16A: 324–328.Google Scholar
- Shin D, Banerjee D: Enhancement of specific heat capacity of high-temperature silica-nanofluids synthesized in alkali chloride salt eutectics for solar thermal-energy storage applications. Int J Heat Mass Tran 2011, 54: 1064–1070. 10.1016/j.ijheatmasstransfer.2010.11.017View ArticleGoogle Scholar
- Tiznobaik H, Shin D: Enhanced specific heat capacity of high-temperature molten salt-based nanofluids. Int J Heat Mass Tran 2013, 57: 542–548. 10.1016/j.ijheatmasstransfer.2012.10.062View ArticleGoogle Scholar
- Cai Y, Ke H, Dong J, Wei Q, Lin J, Zhao Y, Song L, Hub Y, Huang F, Gao W, Fong H: Effects of nano-SiO2 on morphology, thermal energy storage, thermal stability, and combustion properties of electrospun lauric acid/PET ultrafine composite fibers as form-stable phase change materials. Appl Energ 2011, 88: 2106–2112. 10.1016/j.apenergy.2010.12.071View ArticleGoogle Scholar
- Choi SUS: Developments Applications of Non-Newtonian Flows. New York: ASME; 1995.Google Scholar
- Nelson IC, Banerjee D: Flow loop experiments using polyalphaolefin nanofluids. J Thermophys Heat Tran 2009, 23: 752–761. 10.2514/1.31033View ArticleGoogle Scholar
- Zhou LP, Wang BX, Peng XF, Du XZ, Yang YP: On the specific heat capacity of CuO nanofluid. Adv Mech Eng 2010, 2010: 1–4.View ArticleGoogle Scholar
- Vajjha RS, Das DK: Specific heat measurement of three nanofluids and development of new correlations. J Heat Transf 2009, 131: 1–7.View ArticleGoogle Scholar
- Shin D, Banerjee D: Effects of silica nanoparticles on enhancing the specific heat capacity of carbonate salt eutectic (work in progress). Int J Struct Changes Sol 2010, 2: 25–31.Google Scholar
- Shin D, Banerjee D: Enhanced specific heat of silica nanofluid. J Heat Transfer 2011, 133(2):024501–024504. 10.1115/1.4002600View ArticleGoogle Scholar
- O’Hanley H, Buongiorno J, McKrell T, Hu L: Measurement and model validation of nanofluid specific heat capacity with differential scanning calorimetry. Adv Mec Eng 2012, 2012: 181079.Google Scholar
- Buongiorno J: Convective transport in nanofluids. J Heat Transf 2006, 128: 240–250. 10.1115/1.2150834View ArticleGoogle Scholar
- Banerjee SD: Enhanced specific heat capacity of nanomaterials synthesized by dispersing silica nanoparticles in eutectic mixtures. J Heat Transfer 2013, 135(3):032801–032808. 10.1115/1.4005163View ArticleGoogle Scholar
- Lu MC, Huang CH: Specific heat capacity of molten salt-based alumina nanofluids. Nanoscale Res Lett 2013, 8: 292–299. 10.1186/1556-276X-8-292View ArticleGoogle Scholar
- Little F: Molten salt carbon nanotube thermal energy storage for concentrating solar power systems. In DOE Peer Review. Texas A&M University: Space Engineering Research Center; 2011.Google Scholar
- Namburu PK, Kulkarni DP, Dandekar A, Das DK: Experimental investigation of viscosity and specific heat of silicon dioxide nanofluids. Micro Nano Lett 2007, 2: 67–71. 10.1049/mnl:20070037View ArticleGoogle Scholar
- Zhou S-Q, Ni R: Measurement of the specific heat capacity of water-based Al2O3 nanofluid. Appl Phys Lett 2008, 92: 093123. 10.1063/1.2890431View ArticleGoogle Scholar
- Jang SP, Choi SUS: Role of Brownian motion in the enhanced thermal conductivity of nanofluids. Appl Phys Lett 2004, 84: 4316–4318. 10.1063/1.1756684View ArticleGoogle Scholar
- Prasher R, Bhattacharya P, Phelan P: Thermal conductivity of nanoscale colloidal solutions (nanofluids). Phys Rev Lett 2005, 94: 025901.View ArticleGoogle Scholar
- Evans W, Fish J, Keblinski P: Role of Brownian motion hydrodynamics on nanofluid thermal conductivity. Appl Phys Lett 2006, 88(9):093116. 10.1063/1.2179118View ArticleGoogle Scholar
- Evans W, Prasher R, Fish J, Meakin P, Phelan P, Keblinski P: Effect of aggregation and interfacial thermal resistance on thermal conductivity of nanocomposites and colloidal nanofluids. Int J Heat Mass Tran 2008, 51(5):1431–1438.View ArticleGoogle Scholar
- Zhu H, Zhang C, Liu S, Tang Y, Yin Y: Effects of nanoparticle clustering and alignment on thermal conductivities of Fe3O4 aqueous nanofluids. Appl Phys Lett 2006, 89: 023123. 10.1063/1.2221905View ArticleGoogle Scholar
- Xuan Y, Li Q, Hu W: Aggregation structure and thermal conductivity of nanofluids. AlChE Journal 2003, 49(4):1038–1043. 10.1002/aic.690490420View ArticleGoogle Scholar
- Li L, Zhang Y, Ma H, Yang M: Molecular dynamics simulation of effect of liquid layering around the nanoparticle on the enhanced thermal conductivity of nanofluids. J Nanopart Res 2010, 12: 811–821. 10.1007/s11051-009-9728-5View ArticleGoogle Scholar
- Oh SH, Kauffmann Y, Scheu C, Kaplan WD, Rühle M: Ordered liquid aluminum at the interface with sapphire. Science 2005, 310: 661–663. 10.1126/science.1118611View ArticleGoogle Scholar
- Yu W, Choi SUS: The role of interfacial layers in the enhanced thermal conductivity of nanofluids: a renovated Maxwell model. J Nanopart Res 2003, 5: 167–171.View ArticleGoogle Scholar
- Ishida H, Rimdusit S: Heat capacity measurement of boron nitride-filled polybenzoxazine: the composite structure-insensitive property. J Therm Anal Calorim 1999, 58: 497–507. 10.1023/A:1010127805836View ArticleGoogle Scholar
- O’Neill MJ: Measurement of specific heat functions by Differential Scanning Calorimetry. Anal Chem 1966, 36: 1331–1336.View ArticleGoogle Scholar
- Mehling H, Cabeza LF: Heat and cold storage with PCM: An up to date introduction into basics and applications. Berlin: Springer; 2008.Google Scholar
- Anoop K, Sadr R, Yu J, Kang S, Jeon S, Banerjee D: Experimental study of forced convective heat transfer of nanofluids in a microchannel. Int Commun Heat Mass 2012, 39: 1325–1330. 10.1016/j.icheatmasstransfer.2012.07.023View ArticleGoogle Scholar
- Murshed SMS, Leong KC, Yang C: Enhanced thermal conductivity of TiO2-water based nanofluids. Int J Therm Sci 2005, 44(4):367–370. 10.1016/j.ijthermalsci.2004.12.005View ArticleGoogle Scholar
- Wang L, Tan ZC, Meng SH, Liang D, Li GH: Enhancement of molar heat capacity of nanostructured Al2O3. J Nanopart Res 2001, 3: 483–487. 10.1023/A:1012514216429View ArticleGoogle Scholar
- Wang BX, Zhou LP, Peng XF: Surface and size effects on the specific heat capacity of nanoparticles. Int J Thermophys 2006, 27: 139–151. 10.1007/s10765-006-0022-9View ArticleGoogle Scholar
- Saterlie M, Sahin H, Kavlicoglu B, Liu Y, Graeve O: Particle size effects in the thermal conductivity enhancement of copper-based nanofluids. Nanoscale Res Lett 2011, 6(1):217–224. 10.1186/1556-276X-6-217View ArticleGoogle Scholar
- Wu D, Zhu H, Wang L, Liu L: Critical issues in nanofluids preparation, characterization and thermal conductivity. Curr Nanosci 2009, 5: 103–112. 10.2174/157341309787314548View ArticleGoogle Scholar
- Xie H, Wang J, Xi T, Liu Y, Ai F, Wu Q: Thermal conductivity enhancement of suspensions containing nanosized alumina particles. J Appl Phys 2002, 91(7):4568–4572. 10.1063/1.1454184View ArticleGoogle Scholar
- Timofeeva EV, Routbort JL, Singh D: Particle shape effects on thermophysical properties of alumina nanofluids. J Appl Phys 2009, 106: 014304. 10.1063/1.3155999View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an open access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.